Electron Paramagnetic Resonance Investigation of Puriﬁed Catalyst-free Single-Walled Carbon Nanotubes Mujtaba Zaka,† Yasuhiro Ito,† Huiliang Wang,† Wenjing Yan,† Alex Robertson,† Yimin A. Wu,† Mark H. Ru¨mmeli,‡,§ David Staunton,⬜ Takeshi Hashimoto,¶ John J. L. Morton,† Arzhang Ardavan,# G. Andrew D. Briggs,† and Jamie H. Warner†,* †
Department of Materials, University of Oxford, Parks Rd, Oxford, OX1 3PH, United Kingdom, ‡IFW Dresden, P.O. Box 270116, D-01171 Dresden, Germany, §Technische Universita¨t Dresden, Dresden, D-01062, Germany, ⬜Department of Biochemistry, University of Oxford, South Parks Road, Oxford, OX1 3QU, United Kingdom, ¶Meijo Nano Carbon Co. Ltd, 3-4-10 Marunouchi, Naka-ku, Nagoya, 460-0002, Japan, and #Clarendon Laboratory, Department of Physics, University of Oxford, Parks Rd, Oxford, OX1 3PH, United Kingdom
ABSTRACT Electron paramagnetic resonance of single-walled carbon nanotubes (SWCNTs) has been bedevilled by the presence of paramagnetic impurities. To address this, SWCNTs produced by laser ablation with a nonmagnetic PtRhRe catalyst were purified through a multiple step centrifugation process in order to remove amorphous carbon and catalyst impurities. Centrifugation of a SWCNT solution resulted in sedimentation of carbon nanotube bundles containing clusters of catalyst particles, while isolated nanotubes with reduced catalyst particle content remained in the supernatant. Further ultracentrifugation resulted in highly purified SWCNT samples with a narrow diameter distribution and almost no detectable catalyst particles. Electron paramagnetic resonance (EPR) signals were detected only for samples which contained catalyst particles, with the ultracentrifuged SWCNTs showing no EPR signal at X-band (9.4 GHz) and fields < 0.4 T. KEYWORDS: single-walled · nanotubes · electron paramagnetic resonance · ultracentrifugation
arbon nanotubes are ideal for the production of spintronic1 devices owing to the long electron spin lifetimes and high Fermi velocity.2 It is vital to understand the magnetic properties of electrons in single-walled carbon nanotubes (SWCNTs) in order to effectively utilize them in spintronics. Electron paramagnetic resonance (EPR) is an ideal method for providing insights into the spin properties of SWCNTs as it can probe conduction electrons and unpaired spins. EPR of SWCNTs was reported by Petit et al.,3 and a strong signal attributed to conduction electrons was observed. Bandow et al.4 reported experiments on multiwalled nanotubes and SWCNTs that indicated a relationship between contacting nanotube bundles and the EPR line shape. Contrary to the experiment by Petit, no signal associated with the presence of conduction electrons was detected. Salvetat5 irradiated SWCNTs with 2.5 MeV electrons, inducing defects, in order
*Address correspondence to [email protected]
Received for review September 30, 2010 and accepted November 2, 2010. Published online November 17, 2010. 10.1021/nn102602a © 2010 American Chemical Society
VOL. 4 ▪ NO. 12 ▪ ZAKA ET AL.
to detect conduction electron spin resonance. However, the EPR spectrum was dominated by magnetic catalyst impurities. In an attempt to solve this problem of magnetic catalyst particle impurities Corzilius et al.6 used carbon nanotubes grown using chemical vapor deposition (CVD). These vertically aligned forests of nanotubes can be removed from the substrate, leaving behind the residual catalyst. Low temperature measurements found sharp EPR lines that were attributed to conduction electrons trapped inside nanotube defects. However, the lack of in-depth structural characterization by high resolution transmission electron microscopy (HRTEM) makes it difficult to link EPR properties with specific structural features of the SWCNTs. EPR has also been employed to study SWCNT peapod structures7,8 elucidating charge transfer between metallofullerenes and SWCNTs, and hydrogen absorption9 of nanotubes preferentially at defect sites, causing the EPR signal to diminish. These often discordant results of SWCNT EPR highlight the need for ultrapure samples free from metal impurities and the application of multiple characterization techniques in order to build a balanced and deep picture of the structure⫺EPR relationship. SWCNTs have generally been grown using magnetic transition metal catalyst particles,3⫺5 which contribute strong EPR signals, and efforts to remove magnetic particles often leave the SWCNTs highly defective.6 Preparation of high quality pristine SWCNTs are essential for the investigation of the origin of SWCNT EPR. SWCNTs processing requires the removal www.acsnano.org
ARTICLE Figure 1. HRTEM images illustrating the composition of the SWCNT samples through each step in the purification process: (A-i) lowmagnification image of raw laser ablation PtRhRe SWCNTs; (A-ii) high-magnification image of raw SWCNTs showing amorphous carbon coating the nanotube surface; (B-i) low-magnification image of annealed PtRhRe SWCNTs; (B-ii) high-magnification image of annealed SWCNTs showing clean nanotubes and catalyst particles; (C) sonicated PtRhRe SWCNTs coated with surfactant; (D) centrifuged SWCNT supernatant showing a reduction in catalyst particles; (E) low-magnification image of centrifuged SWCNT sediment showing large clusters of catalyst particles; (F) HRTEM image of DGU treated SWCNTs showing minimal catalyst particle content.
of amorphous carbon and catalyst particles with minimal damage to the nanotube structure. Here, we utilize two different purification methods to remove amorphous and graphitic carbon, and catalyst particle impurities, based upon high vacuum high thermal annealing and ultracentrifugation.10,11 Kitaura et al.10 annealed raw SWCNTs at 1200 °C for 24 h under high vacuum to remove amorphous carbon and vaporize Fe catalyst particles. Superconducting quantum interference device (SQUID) magnetometry of the thermally annealed SWCNT sample showed minimal magnetic susceptibility over the temperature range, demonstrating the removal of Fe catalyst particles while retaining nanotube structure. Ultracentrifugation allows for facile separation of nanotubes and catalyst particles without damaging the carbon nanotube structure. Density gradient ultracentrifugation (DGU) has been developed as a large scale method for the separation of SWCNTs into semiconducting and metallic chiralities, primarily focusing on smaller diameter nanotubes.12,13 Larger diameter SWCNTs are more challenging to separate into different chiral forms due to the broad overlap of diameter for semiconducting and metallic species. We have concentrated on larger diameter SWCNTs because they can be filled with spin-active metallofullerenes to form 1D peapod systems.7 www.acsnano.org
RESULTS AND DISCUSSION Nanotube Composition. HRTEM was performed to image the composition of all SWCNT samples in each of the purification methods, comparing the nanotube structure and the level of catalyst particles, amorphous carbon and defects present. Figure 1 panels a-i and a-ii show the HRTEM images from the raw PtRhRe SWCNTs containing catalyst particles, amorphous and graphitic carbon. The SWCNTs were annealed in air at 300 °C for 2 h to remove the carbon impurities. Figure 1 panels b-i and b-ii show the annealed PtRhRe SWCNTs with reduced amounts of amorphous carbon either on the surface of the nanotube or surrounding the catalyst particles. A solution of annealed SWCNTs in 2% SC/DOC [4:1 ratio] was prepared and then sonicated for 4 h. HRTEM presented in Figure 1c shows SWCNTs and catalyst particles coated with surfactant. The sonicated SWCNT sample was centrifuged for 1 h at 41 krpm, resulting in the supernatant (top 85%) containing dilute SWCNT solution with the bottom containing a residue of sediment SWCNTs. The “supernatant SWCNT”, Figure 1D, shows a reduction in the amount of catalyst particles and more isolated SWCNTs. In contrast, Figure 1E, the “sediment SWCNT” sample, showed considerable increase in the level of catalyst particles. The supernatant SWCNT sample was further purified through a 17 h ultracentrifugation using a 20⫺40% iodixanol density gradient based upon the DGU method explained in ref VOL. 4 ▪ NO. 12 ▪ 7708–7716 ▪ 2010
diameter distribution and purity of SWCNTs in the ultracentrifugation purification process. UV⫺vis absorption of SWCNT films between 400⫺2200 nm showed two semiconducting peaks, around S11 ⫽ 1900 nm and S22 ⫽ 1050 nm, and the first metallic peak, around M11 ⫽ 700 nm (see Supporting Information). For comparative analysis, the full width half-maximum (fwhm) diameter distribution, calculated using Kataura plot,18 and the relative purity obtained from the S22 peak was examined for all samples (shown in Figure 3a). The mean diameter remained consistent, approximately ⬃1.45 nm, for all SWCNT samples in the purification process. The SWCNT sediment has the broadest fwhm diameter distribution, shown in Figure 3b, while the SWCNT supernatant and DGU SWCNT material have narrower fwhm diameter distribution. Surprisingly the SWCNT sediment and sonicated SWCNT contain narrow nanotubes with diameters ⬍ 1.2 nm. These narrow diameter nanotubes may bundle together and cause them Figure 2. (A) Low-magnification HRTEM image of aqua regia treated SWCNTs showing to sediment. Centrifugation of SWCNT soluclean nanotube bundle with some catalyst particles; (B-i) HRTEM image of Meijo SO tions should force heavy nanotube bundles SWCNTs showing a residual catalyst particle, highlighted with dotted circle; (B-ii) high magnification HRTEM of highlighted catalyst particle showing lattice fringes; (C) lowto sediment, and isolated nanotubes to form magnification HRTEM image of large bundles of Meijo FHP NTs with no visible catalyst in the supernatant. SWCNT purity is a meaparticles; (D) HRTEM image of Meijo FHP NTs refluxed in HNO3, showing bundles of NTs sure of the absorption of SWCNT against immaintaining pristine structure. purities in the sample as explained in ref 12. The resulting sample, Figure 1F, contains many iso19. Relative to the sonicated SWCNT sample the purity lated SWCNTs with almost no visible catalyst particles. increases for the centrifuged supernatant and DGU The centrifuge purification process has been developed SWCNT sample, which has the highest relative purity. as an alternative method to the currently employed The sediment SWCNT sample has the lowest relative aqua regia purification method.7,14,15 Aqua regia inpurity, which is reflective of the high levels of catalyst volves harsh acid treatment to remove the catalyst par- particles as illustrated in the HRTEM, Figure 1E. Meijo ticles, but, as shown in Figure 2a, a significant amount FHP CNTs produced a broad UV⫺vis absorption specof catalyst particles remains. Hot thermal annealing tra due to a very large diameter distribution, therefore has been previously employed as a purification method a fwhm and purity could not be determined. for arc-discharge nanotubes.16 HRTEM of Meijo SO Structural Analysis. Atomic force microscopy (AFM) proSWCNTs, shown in Figure 2b, indicates the presence of vided a further insight into the affect of the centrifugasome residual catalyst particles. Figure 2c shows the HR- tion purification process on the length and bundling of TEM image of Meijo FHP CNTs with a combination of the PtRhRe SWCNTs. HRTEM only provides a qualitasingle-walled and double-walled nanotubes and almost tive idea of the length distribution of the SWCNTs no magnetic catalyst particles. Several hours were spent samples, so it is important to use AFM as an additional using TEM to scan a region of more than 0.01 mm2 of analytical technique. AFM of raw PtRhRe SWCNT, centriFH-P SWNT networks that was found to be catalyst free. fuged SWCNT supernatant, and Meijo FHP SWCNT are The Meijo FHP NTs were refluxed in HNO3 for 2.5 h in or- shown in Figure 4 panels a, b, and c, respectively, and der to produce defects;17 Figure 2d shows the refluxed analyzed in Figure 4d,e. All samples were prepared in Meijo FHP sample still retaining its nanotube structure 2% SC/DOC [4:1 ratio] solution and to ensure good disand no magnetic particles visible. persions raw PtRhRe SWCNTs and Meijo FHP CNTs were Purity Analysis Using Absorption Spectroscopy. Van-Hove sonicated for 1 h. Raw PtRhRe SWCNTs have a mean singularities in SWCNTs produce distinctive absorption length of 1.41 m and the majority of nanotubes with peaks from semiconducting and metallic transitions. length between 1 and 2 m. For the SWCNT supernaUV⫺vis absorption spectroscopy was used to measure tant the distribution of nanotube lengths peaks at the absorption peaks from the metallic and semicon0.5⫺1 m with an average nanotube length of 0.77 m. The shorter nanotube length is due to the 4 h hornducting SWCNTs and yield information regarding the VOL. 4 ▪ NO. 12 ▪ ZAKA ET AL.
VOL. 4 ▪ NO. 12 ▪ 7708–7716 ▪ 2010
Electron Paramagnetic Resonance. X-Band CW EPR measurements for each of the SWCNT species in the centrifugation purification process were performed at 5 K using microwave power of ⬃1 mW (well below the saturation power of ⬃2 mW). EPR samples were prepared with a similar quantity of SWCNTs in order to compare the relative number of spins. Figure 5 compares the EPR intensity of the various SWCNT samples. Raw PtRhRe SWCNTs, Figure 5a, gave a strong single peak in the EPR, with a g-factor of 2.0034 ⫾ 0.0005 and line width ⬇ 3.0 ⫾ 0.1 G, but when the SWCNTs were annealed this signal was no longer detected. We attribute this loss of EPR signal to the removal of amorphous carbon in the annealing process. Centrifugation of the sonicated PtRhRe SWCNT sample decreased the catalyst content and improved the purity of the SWCNT supernatant sample compared to the SWCNTs sediment. The sonicated and Figure 3. (a) UVⴚvis absorption showing the normalized S22 peak for the SWCNTs sedimented SWCNT samples sample, indicating the fwhm for each sample; (b) fwhm diameter distribution (red) and relative purity (blue) relative to sonicated SWCNTs sample for SWCNTs samples, with the show an EPR signal, Figure 5b, S22 peak used as a comparison for all samples. with a Lorentzian line shape and similar linewidths of ⬃5.0 tip sonication of the nanotube which is known to cut ⫾ 0.1 G. The g-factor for sonicated and sediment 20,21 and shorten SWCNTs. The height profile distribuSWCNTs are 2.0029 ⫾ 0.0005 and 2.0017 ⫾ 0.0005, retion for raw PtRhRe peaks between 2 and 4 nm (i.e., spectively. The marginal difference is possibly due to bundles), compared to the lower value of the SWCNTs bundling of nanotubes in the SWCNT sediment. The supernatant, with the majority of the height profile discentrifuged supernatant shows negligible EPR signal tribution less than 2 nm. This indicates that the SWCNT with a similar g-factor of 2.0026 ⫾ 0.0005 and line width supernatant contains principally isolated nanotubes, of ⬃5.0 ⫾ 0.1 G. We can deduce that the EPR signal is which is a direct result of the surfactant encapsulation linked to the presence of catalyst particles present in and centrifugation of the SWCNT. Meijo FHP CNTs are the sonicated and sediment samples. DGU SWCNTs much shorter in length than Raw PtRhRe SWCNTs, with showed minimal EPR signal, further indicating that the a mean length of 0.57 m. Meijo FHP CNTs have a observed EPR signal is related to the presence of catalarger height profile distribution compared to raw lyst particles. SWCNTs purified by aqua regia microwave PtRhRe SWCNT, due to the larger diameter of the Meijo digestion have been shown to contain catalyst parFHP CNTs and the presence of both single-walled and ticles through HRTEM (Figure 3a). Figure 5b shows the double-walled nanotubes. AFM data indicate that both EPR signal of the aqua-regia-treated SWCNTs, which is supernatant SWCNTs and Meijo FHP NTs have sufficient similar to the signal of the sonicated and sediment catamean length to produce isolated NT field effect transis- lyst containing SWCNTS, emphasizing the relationship tor (FET) devices as explained in ref 22. Percolated net- between the catalyst particle impurities and EPR. works of short NTs, ⬃200 nm mean length, have been Figure 6a shows the observed EPR from Meijo SO SWCNTs, Meijo FHP, and refluxed Meijo FHP CNTs. Low employed to produce thin film transistors.23
ARTICLE Figure 4. (A) AFM image of raw PtRhRe SWCNTs; (B) AFM image of SWCNTs supernatant; (C) AFM image of Meijo FHP nanotubes; (D) distribution of nanotube length for nanotube samples; (E) height profile distribution of nanotubes.
temperature (5 K) EPR measurements of Meijo SO SWCNTs show a large single peak with Lorentzian line shape and a g-factor of 2.0012 ⫾ 0.0005 and ⬃5.1 ⫾ 0.1 G line width. This EPR signal can be attributed to the presence of residual magnetic catalyst particles. Meijo FHP CNTs have negligible magnetic catalyst particle content and contain a combination of primarily
Figure 5. (A) 5 K EPR spectra of raw PtRhRe SWCNTs; (B) 5 K EPR spectra of annealed, sonicated, sediment, supernatant, DGU, and aqua regia SWCNTs (microwave power, 1 mW; modulation frequency, 100 kHz; modulation amplitude, 1 G).
VOL. 4 ▪ NO. 12 ▪ ZAKA ET AL.
SWCNTs and some double- and triple-walled nanotubes and show no observable EPR signal. This further supports the notion that the SWCNT EPR signals observed at X-band are linked to the presence of catalyst particles. Meijo FHP NTs are clean catalyst-free graphitic systems, differing from DGU SWCNTs as they are larger in diameter and contain double-walled and triplewalled nanotubes. Since no EPR signal is observed at the X-band for either nanotube sample, this suggests that changes in nanotube diameter and the number of walls do not produce an observable X-band EPR signal. Meijo FHP CNTs were refluxed to induce defects into the nanotube structure. The refluxed Meijo FHP CNTs showed no EPR signal at low temperature, similar to the raw Meijo FHP sample, indicating the minimal effect of defects on the EPR signal. To further confirm the notion that ultrapure SWCNTs do not produce an observable signal in low temperature (5 K) EPR at X-band, we examined 95% purified semiconducting and 95% purified metallic SWCNT samples produced by Nanointegris using the DGU method.12 No signal was observed from these samples as shown in Figure 6b. To our knowledge this is the first report of the EPR examination of pure metallic (and semiconducting) SWCNTs. This reveals that the EPR associated with possible conduction electrons is not seen at X-band and may require larger field strengths and higher microwave frequencies. This is highly challenging and is the subject of our further work. Vibrating Sample Magnetometry. A vibrating sample magnetometer (VSM) was used to characterize the magnetic properties of the nanotube samples by measuring any magnetization arising from magnetic catalyst www.acsnano.org
VOL. 4 ▪ NO. 12 ▪ 7708–7716 ▪ 2010
D peaks of the SWCNT samples to determine any effects the centrifugation purification process had upon SWCNT defects. The ratio of the D peak (⬃1330 cm⫺1), defects in sp2 carbon network, and the G peak (⬃1590 cm⫺1), arising from semiconducting and metallic nanotubes, is used to measure the degree of disorder in the SWCNTs.25 Similar D/G ratios were obtained for DGU SWCNTs, 0.059, and raw SWCNTs, 0.058, while smaller D/G ratios were obtained for aqua-regia-treated SWCNTs, 0.028, and Meijo SO SWCNTs, 0.032. The D peak for DGU SWCNTs may be slightly higher due to the horn-tip sonication process which may create defects through the process of cutting nanotubes. The relatively low D/G ratio for all the SWCNTs samples illustrates the high quality of the SWCNTs.25,26 Paramagnetic Properties. Purified DGU SWCNTs and Meijo FHP NTs free from catalyst particles show negligible EPR signals at X-band. EPR signals were only detected in samples containing catalyst particles indicating there may be some interactions between the metal catalyst and surrounding carbon which contributes to the EPR signal. Nicolau et al.27 investigated the paramagnetic behavior of platinum catalyst deposited on charcoal. They investigated sevFigure 6. (A) The 5 K EPR of Meijo SO (dashed), Meijo FHP (solid), and refluxed Meijo FHP (dotted); (B) 5 K EPR of metallic SWCNT eral compositions of platinum and charcoal and (blue) and semiconducting SWCNT (purple) (microwave power, found that mixed Pt⫺C complexes produced EPR 1 mW; modulation frequency, 100 kHz; modulation amplitude, signals, with linewidths between 3.9 and 5.4 G and 1 G). a g-factor of 2.0034, around that of a free electron particles and to further demonstrate that Meijo FHP and similar to the observed g-factors in Figures 5 and nanotube were free from magnetic catalyst particles. 6. The observed EPR signal was attributed to interaction Figure 7a shows the VSM of raw PtRhRe, Meijo FHP, and between charcoal and the platinum, and a relationship Meijo SO SWCNTs. The PtRhRe catalyst particles are between the EPR intensity and platinum content was nonmagnetic and therefore no magnetization curve is observed, indicating that electrons remain unpaired on observed in the VSM. Meijo SO and FHP CNTs are synthe platinum catalyst. These observations facilitate an thesized using ferromagnetic catalysts, Ni/Y and Fe, re- understanding of the obtained EPR signals in our exspectively, and undergo high vacuum thermal annealperiments. Annealing raw PtRhRe SWCNTs removes ing with the aim of removing catalyst particles.16 Meijo amorphous carbon surrounding the nanotube and SO SWCNTs are single-walled and have a similar diamcatalyst particle surface. The cleansed catalyst particles eter distribution to raw PtRhRe SWCNTs. The VSM of no longer form Pt⫺C interactions with the removed Meijo SO SWCNTs shows trace amounts of catalyst par- amorphous carbon, explaining the absence of an obticles, as determined by the weak hysteresis curve. As servable EPR signal for annealed SWCNTs. Wang et al.28 a comparison, the inset in Figure 7a shows the VSM of performed density functional theory (DFT) calculations Carbolex SWCNTs heavily coated with ferromagnetic to ascertain the binding energies of Pt clusters on carcatalyst particles; the strong hysteresis curve is indicabon nanotubes. Binding energies on point defects on tive of the presence of soft magnetic catalyst particles CNTs were determined to be more than three times (cf. ref 24). Meijo FHP nanotubes are of a larger diamhigher than on defect-free CNTs. Stronger orbital hyeter and contain single-walled and double-walled nano- bridization between Pt atoms and carbon in defective tubes. They are more stable to higher temperatures for CNTs was determined to cause the increase in the bindannealing, resulting in maximum removal of magnetic ing energy. Importantly Wang et al. elucidated that catalyst particles; they therefore show no magnetic sig- larger charge transfer occurred between Pt and carbon nals in VSM. These observations account for the origin in defect CNTs. Sonication of SWCNT surfactant solution of the detected EPR signal in Meijo SO SWCNTs, which has been shown to cut nanotubes, and Lu et al. elucicontain magnetic catalyst particles, and the absence of dated the mechanical damage that can potentially arise any EPR signal for catalyst particle-free Meijo FHP NTs. from ultrasonication, producing defects in the nanoRaman Spectroscopy. Raman spectroscopy, shown in Fig- tube structure.21,28,29 Shorter nanotubes with potential ure 7b, was performed at 532 nm to measure the G and defects could provide more preferential binding sites
shown to be a pure graphitic system, an ideal nanotube structure which has been lacking in preceding EPR studies, and shows no trace of conduction electrons. Theoretical calculations predict a doublet peak for SWCNTs EPR due to spin⫺charge separation; however, neither of our purified samples show this phenomenon at X-band.30 Kuemmeth et al.31 measured spin orbital coupling of 84 GHz for a single 5 nm diameter SWCNT.31 On the basis of their measurement of the spin orbit (SO) coupling and theoretical study of ref 32, we can estimate a SO coupling for the nanotubes studied here (DGU SWCNTs diameter ⬇ 1.4⫺1.6 nm, and Meijo FHP NTs, diameter ⬇ 2 nm) to be approximately 260⫺300 GHz and 190⫺230 GHz, respectively. Given these values for SO coupling, we would expect no EPR signal from the conduction electrons at X-band (10 GHz) and at a modest magnetic field. Furthermore the range of nanotube diameters could lead to substantial broadening and therefore make it difficult to observe any signal. Studying aligned SWCNTs at higher EPR frequencies could reveal the conduction electron spin resonance. SUMMARY The multistep centrifugation purification process has successfully produced highly pure SWCNTs which can be implemented in spintronic devices. Centrifugation of SWCNT solutions provides an effective approach to removing catalyst particles compared to aqua regia treatment. HRTEM, UV⫺vis, and AFM provided Figure 7. (A) VSM of raw PtRhRe (circle), Meijo FHP (square), and Meijo SO (trievidence for the significant improvement of the angle) SWCNTs. (Inset) VSM of Carbolex raw SWCNTs containing many catalyst SWCNTs through each step in the purification particles. (B) Raman spectroscopy of Raw SWCNTs, DGU SWCNTs, aqua regia SWCNTs, and Meijo SO SWCNTs showing the G peak (⬃1590 cmⴚ1) and D peak process. EPR tracked any modifications the pu(⬃1340 cmⴚ1). rification methodology had on the SWCNTs sample. The comparative analysis of the sedifor Pt catalyst particles to interact with the CNT and pro- ment and supernatant SWCNT samples has revealed vide an explanation of the reappearance of an EPR sig- that metal catalyst carbon complexes were the cause nal for the sonicated SWCNTs sample. We centrifuged of the observable EPR signal. the sonicated SWCNT sample, producing two SWCNTs HRTEM and UV⫺vis established the difference besystems with varying Pt catalyst content, as determined tween the two samples, the SWCNT sediment conby HRTEM. An EPR signal is observed for sediment taining a substantial amount of catalyst particles and SWCNTs, heavily coated with catalyst particles, due to the SWCNT supernatant containing more isolated the Pt⫺C interactions. Supernant and DGU SWCNTs, SWCNTs with considerable reduction in catalyst parcontaining predominantly nanotubes, yielded no obticle content and a narrower diameter distribution. servable EPR signals at X-band due to the absence of EPR of the two contrasting SWCNT samples highPt⫺C interactions. Observed EPR signals arise from the lights a strong correlation between the level of catainteraction between the Pt catalyst particle and the lyst particles and the detected EPR signal. Purified CNTs, and centrifugation has successfully demonstrated supernatant and DGU SWCNTs show no EPR signal an avenue to reduce catalyst content from the nanoat X-band, whereas the sonicated and sediment tube system.26,27 High vacuum thermal annealing of SWCNTs, containing higher levels of catalyst parmagnetic catalyst particles from Meijo FHP CNTs highticles, both produced an EPR signal. Since aqualighted another approach to remove catalyst particles, regia-purified SWCNTs contain residual catalyst parwhich otherwise produce an EPR signal as seen for ticles they therefore produce an EPR signal. Ultracentrifugation of raw PtRhRe is a viable method Meijo SO SWCNTs.10,16 Meijo FHP CNTs have been
VOL. 4 ▪ NO. 12 ▪ ZAKA ET AL.
METHODS SWCNTs were grown using laser ablation with nonmagnetic catalyst particles (PtRhRe) using a previously reported method.14 Purification to remove catalyst content was performed either by aqua-regia microwave digestion or through centrifugation.15 Centrifugation involved multiple steps to purify the raw PtRhRe SWCNTs, as shown in the schematic diagram in Figure 8. The SWCNTs were annealed in air at 300 °C for 2 h in order to remove amorphous carbon. Annealed SWCNTs were dispersed in an aqueous solution of 2% sodium cholate (SC)/deoxy cholate (DOC) [ratio 4:1] to a concentration of 0.5 mg mL⫺1. The SWCNT 2% SC/DOC solution was sonicated for 4 h using a horn-tip sonicator (Cole Parmer ultrasonic processor). The sample was placed in an ice bath to prevent thermal damage to the SWCNTs. The sonicated SWCNT solution was centrifuged for 1 h at 41 krpm using a swing bucket SW41Ti rotor and Beckman Coulter ultracentrifuge model L100-XP. The upper 85% of the solution was collected and is termed “SWCNT supernatant”. The material at the bottom of the centrifuge tube was also collected and is termed “SWCNT sediment”. The SWCNT supernatant was concentrated using centrifugal filters (Amicon 30 kDa, Millipore), for 7 min at 5 krpm, (Labofuge 200 Heraues). The concentrated SWCNT supernatant sample was further centrifuged for 17 h at 41 krpm using an iodixanol density gradient (20⫺40% linear gradient with 2% sodium cholate/sodium dodecyl sulfate [ratio 2:3]). The process of using density gradient ultracentrifugation (DGU) is employed with the primary function of isolating catalyst-free SWCNTs. The separated fractions from the DGU were isolated, and the bulk black nanotube suspension was collected and termed “DGU SWCNT”. Meijo FHP and SO SWCNTs were produced by Meijo Nano Carbon, Inc, via arc-discharge using magnetic catalyst particles Fe and Ni/Y, respectively. As-grown arc-discharge SWCNTs were air oxidized at 400 °C and further purified in hydrochloric acid. High temperature annealing was performed between 1100⫺1400 °C at a vacuum pressure of 10⫺3⫺10⫺4 Pa for 6⫺24 h. To understand the affect of nanotube defects on the EPR signal Meijo FHP SWCNTs were refluxed in nitric acid HNO3 for 2.5 h at 130 °C in order to induce defects. DGU separated ultrapure semiconducting (IsoNanotube-S) and metallic (IsoNanotube-M) SWCNT buckypapers (95% purified) for EPR analysis were purchased from Nanointegris.
to obtain catalyst-free SWCNTs. Meijo SO and FHP NTs illustrate analogous results. High thermal annealing of Meijo FHP NTs purged magnetic catalyst particles, as shown in VSM, whereas Meijo SO show the presence of magnetic particles in VSM. Meijo FHP nanotubes are highly pure, with HRTEM and VSM giving no indication of any catalyst particle present in Figure 8. Schematic diagram indicating the multiple steps involved in the purification process of the SWCNTs. the sample. The presence of catalyst particles in Meijo SO is demonstrated X-band either. We can conclude that in general highin the EPR in Figure 6a, with the magnetic catalystquality ultrapure SWNTs do not exhibit an EPR sigfree Meijo FHP CNTs showing no EPR signal. Ultranal at the X-band and that signals detected arise pure DGU separated metallic and semiconducting from metal catalyst particles interacting with carSWNTs did not show any detectable EPR signal at the bon or in poor quality SWNT samples.
UV⫺vis absorption spectroscopy was measured for SWCNT films between 400 and 2200 nm using a Jasco V-570 UV/vis/NIR spectrometer. Vibration sample magnetometer measurements were performed using a Lakeshore 7400 VSM and EM4-HVA electromagnet. Atomic force microscopy (AFM) was performed using a Park Scientific instrument CP-II AFM. AFM samples were prepared by spin coating SWCNT solutions on functionalized Si/SiO substrates.33 For high resolution transmission electron microscopy (HRTEM), SWCNT solutions were washed with methanol, and this washing repeated 5 times to ensure that the surfactant was removed. HRTEM was performed on a JEOL 4000EX operating at 80 kV. All samples for EPR were pumped to remove oxygen and sealed in a quartz tube under vacuum. EPR measurements were performed using a Bruker EMX spectrometer at 9.4 GHz at 5 K in an Oxford ESR900 cryostat. Raman spectroscopy was measured using a JY Horiba Labram Aramis Raman microscope using a frequency doubled Nd:YAG laser at 532 nm. Acknowledgment. J.H.W. is supported by the Glasstone Fund and Brasenose College, Oxford. A.A. and J.J.L.M are supported by the Royal Society. G.A.D.B. thanks EPSRC, IMPRESS, (GR/ S15808/01). M.H.R. thanks the EU (ECEMP) and the Freistaat Sachsen. Supporting Information Available: UV⫺vis absorption of SWCNT films between 400⫺2200 nm. This material is available free of charge via the Internet at http://pubs.acs.org.
REFERENCES AND NOTES 1. Zutic´, I.; Fabian, J.; Das Sarma, S. Spintronics: Fundamentals and Applications. Rev. of Mod. Phys. 2004, 76, 323–410. 2. Hueso, L. E.; Pruneda, J. M.; Ferrari, V.; Burnell, G.; ValdesHerrera, J. P.; Simons, B. D.; Littlewood, P. B.; Artacho, E.; Fert, A.; Mathur, N. D. Transformation of Spin Information into Large Electrical Signals Using Carbon Nanotubes. Nature 2007, 445, 410–413. 3. Petit, P.; Jouguelet, E.; Fischer, J. E.; Rinzler, A. G.; Smalley, R. E. Electron Spin Resonance and Microwave Resistivity of Single-Wall Carbon Nanotubes. Phys. Rev. B 1997, 56, 9275–9278.
VOL. 4 ▪ NO. 12 ▪ 7708–7716 ▪ 2010
4. Bandow, S.; Asaka, S.; Zhao, X.; Ando, Y. Purification and Magnetic Properties of Carbon Nanotubes. Appl. Phys. A 1998, 67, 23–27. 5. Salvetat, J. P.; Feher, T.; L’Huillier, C.; Beuneu, F.; Forro, L. Anomalous Electron Spin Resonance Behaviour of SingleWalled Carbon Nanotubes. Phys. Rev. B 2005, 72, 075440. 6. Corzilius, B.; Gembus, A.; Weiden, N.; Dinse, K. P.; Hata, K. EPR Characterization of Catalyst-free SWNT and [email protected]
Peapods. Phys. Stat. Sol. (b) 2006, 243, 3273–3276. 7. Zaka, M.; Warner, J. H.; Ito, Y.; Morton, J. J. L.; Ru¨mmeli, M. H.; Pichler, T.; Ardavan, A.; Shinohara, H.; Briggs, G. A. D. Exchange Interactions of Spin-Active Metallofullerenes in Solid-State Carbon Networks. Phys. Rev. B. 2010, 81, 075424. 8. Na´fra´di, B.; Nemes, N. M.; Fehe´r, T.; Forro´, L.; Kim, Y.; Fischer, J. E.; Luzzi, D. E.; Simon, F.; Kuzmany, H. Electron Spin Resonance of Single-Walled Carbon Nanotubes and Related Structures. Phys. Stat. Sol. (b) 2006, 243, 3106–3110. 9. Shen, K.; Tierney, D. L.; Pietra␤, T. Electron Spin Resonance of Carbon Nanotubes Under Hydrogen Adsorption. Phys. Rev. B. 2003, 68, 165418. 10. Kitaura, R.; Ogawa, D.; Kobayashi, K.; Saito, T.; Ohshima, S.; Nakamura, T.; Yoshikawa, H.; Awaga, K.; Shinohara, H. High Yield Synthesis and Characterization of the Structural and Magnetic Properties of Crystalline ErCl3 Nanowires in Single-Walled Carbon Nanotube Templates. Nano Res. 2008, 2, 152–157. 11. Nishide, D.; Miyata, Y.; Yanagi, K.; Tanaka, T.; Kataura, H. Effective Separation of Carbon Nanotubes and Metal Particles from Pristine Raw Soot by Ultracentrifugation. Jpn. J. Appl. Phys. 2009, 48, 015004. 12. Arnold, M. S.; Green, A. A.; Hulvat, J. F.; Stupp, S. I.; Hersam, M. C. Sorting Carbon Nanotubes by Electronic Structure using Density Differentiation. Nat. Nanotechnol. 2006, 1, 60–65. 13. Yanagi, K.; Miyata, Y.; Kataura, H. Optical and Conductive Characteristics of Metallic Single-Wall Carbon Nanotubes with Three Basic Colors; Cyan, Magenta, and Yellow. Appl. Phys. Exp. 2008, 1, 034003. 14. Ru¨mmeli, M. H.; Kramberger, C.; Lo¨ffler, M.; Jost, O.; Bystrzejewski, M.; Gru¨neis, A.; Gemming, T.; Pompe, W.; Bu¨chner, B.; Pichler, T. Catalyst Volume to Surface Area Constraints for Nucleating Carbon Nanotubes. J. Phys. Chem. C 2007, 111, 8234–8241. 15. Scho¨nfelder, R.; Ru¨mmeli, M. H.; Gruner, W.; Lo¨ffler, M.; Acker, J.; Hoffmann, V.; Gemming, T.; Bu¨chner, B.; Pichler, T. Purification-Induced Sidewall Functionalization of Magnetically Pure Single-Walled Carbon Nanotubes. Nanotechnology 2007, 18, 375601. 16. Zhao, X.; Inoue, S.; Jinno, M.; Suzuki, T.; Ando, Y. Macroscopic Oriented Web of Single-Wall Carbon Nanotubes. Chem. Phys. Lett. 2003, 373, 266–271. 17. Hu, H.; Zhao, B.; Itkis, M. E.; Haddon, R. C. Nitric Acid Purification of Single-Walled Carbon Nanotubes. J. Phys. Chem. B 2003, 107, 13838–13842. 18. Kataura, H.; Kumazawa, Y.; Maniwa, Y.; Umezu, I.; Suzuki, S.; Ohtsuka, Y.; Achiba, Y. Optical Properties of Single-Wall Carbon Nanotubes. Synth. Met. 1999, 103, 2555–2558. 19. Itkis, M. E.; Perea, D. E.; Niyogi, S.; Rickard, S. M.; Hamon, M. A.; Hu, H.; Zhao, B.; Haddon, R. C. Purity Evaluation of As-Prepared Single-Walled Carbon Nanotube Soot by Use of Solution-Phase Near-IR Spectroscopy. Nano Lett. 2003, 3, 309–314. 20. Yudasaka, M.; Zhang, M.; Jabs, C.; Iijima, S. Effect of an Organic Polymer in Purification and Cutting of Single-Wall Carbon Nanotubes. Appl. Phys. A 2000, 71, 449–451. 21. Shelimov, K. B.; Esenaliev, R. O.; Rinzler, A. G.; Huffman, C. B.; Smalley, R. E. Purification of Single-Wall Carbon Nanotubes by Ultrasonically Assisted Filtration. Chem. Phys. Lett. 1998, 282, 429–434. 22. Cantone, A. L.; Buitelaar, M. R.; Smith, C. G.; Anderson, D. G.; Jones, A. C.; Chorley, S. J.; Casiraghi, C.; Lombardo, A.;
VOL. 4 ▪ NO. 12 ▪ ZAKA ET AL.
Ferrari, A. C.; Shinohara, H.; et al. Electronic Transport Characterization of [email protected]
Single-Wall Carbon Nanotube Peapods. J. Appl. Phys. 2008, 104, 083717. Asada, Y.; Miyata, Y.; Ohno, Y.; Kitaura, R.; Sugai, T.; Mizutani, T.; Shinohara, H. High-Performance Thin-Film Transistors with DNA-Assisted Solution Processing of Isolated Single-Walled Carbon Nanotubes. Adv. Mater. 2010, 22, 2698–2701. Scha¨ffel, F.; Ta¨schner, C.; Ru¨mmeli, M. H.; Neu, V.; Wolff, U.; Queitsch, U.; Pohl, D.; Kaltofen, R.; Leonhardt, A.; Rellinghaus, B.; et al. Carbon Nanotubes Terminated with Hard Magnetic FePt Nanomagnets. Appl. Phys. Lett. 2009, 94, 193107. Eklund, P. C.; Holden, J. M.; Jishi, R. A. Vibrational Modes of Carbon Nanotubes; Spectroscopy and Theory. Carbon 1995, 33, 959–972. Dennany, L.; Sherrell, P.; Chen, J.; Innis, P. C.; Wallace, G. G.; Minett, A. I. EPR Characterisation of Platinum Nanoparticle Functionalised Carbon Nanotube Hybrid Materials. Phys. Chem. Chem. Phys. 2010, 12, 4135–4141. Nicolau, C. S.; Thom, H. G.; Pobitschka, E. Electron Spin Resonance Studies of some Supported Hydrogenation⫺Dehydrogenation Catalysts. Trans. Faraday Soc. 1959, 55, 1430–1434. Wang, J.; Lv, Y.; Li, X.; Dong, M. Point-Defect Mediated Bonding of Pt Clusters on (5,5) Carbon Nanotubes. J. Phys. Chem. C. 2009, 113, 890–893. Lu, K. L.; Lago, R. M.; Chen, Y. K.; Green, M. L. H.; Harris, P. J. F.; Tsang, S. C. Mechanical Damage of Carbon Nanotubes by Ultracentrifugation. Carbon 1996, 34, 814– 816. De Martino, A.; Egger, R.; Hallberg, K.; Balseiro, C. A. SpinOrbit Coupling and Electron Spin Resonance Theory for Carbon Nanotubes. Phys. Rev. Lett. 2002, 88, 206402. Kuemmeth, F.; Ilani, S.; Ralph, D. C.; McEuen, P. L. Coupling of Spin and Orbital Motion of Electrons in Carbon Nanotubes. Nature 2008, 452, 448–452. Huertas-Hernando, D.; Guinea, F.; Brataas, A. Spin-Orbit Coupling in Curved Graphene, Fullerenes, Nanotubes, and Nanotube Caps. Phys. Rev. B 2006, 74, 155426. Liu, J.; Casavant, M. J.; Cox, M.; Walters, D. A.; Boul, P.; Lu, W.; Rimberg, A. J.; Smith, K. A.; Colbert, D. T.; Smalley, R. E. Controlled Deposition of Individual Single-Walled Carbon Nanotubes on Chemically Functionalized Templates. Chem. Phys. Lett. 1999, 303, 125–129.